1 Per. Mineral. (1999), 68, 1, 1-11 [';\] PERIODICO di MINERALOGIA established in 1930 An Intemational Journal of MINERALOGY, CRYSTALLOGRAPHY, GEOCHEMISTRY, ORE DEPOSITS, PETROLOGY, VOLCANOLOGY and applied topics on Environment, Archaeometry and Cultural Heritage The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials ALESSANDRO F. GUALTIERI* Dipartimento di Scienze della Terra, Universita di Modena e Reggio Emilia, ViaS. Eufemia 19, Modena, Italy Submitted, January Accepted, Februmy 1999 ABSTRACT. - Fibrous asbestos minerals have been identified as priority substances for risk reduction and pollution prevention. Because of the well known hazardous effects associated with past occupational exposures to asbestos and because of its widespread use in commerce, exposures to asbestos present a general health hazard. Therefore, the identification and quantification of asbestos in bulk materials which are still sited in a number of plants and public buildings is fundamental for a proper plan of social prevention and general intervention. X-ray powder diffraction is considered an effective tool of investigation of bulk materials with a high statistical significance. The combined Rietveld-RIR method, has been successfully applied for the quantitative determination in the past of asbestos in bulk materials such as insulating cements, mixed asbestos-slag wools, contaminated soils, and others. The University of Jussieu in Paris has been partly evacuated because the framework of the building is composed of an asbestos rich material. This paper reports the description of the characterisation of that material and a possible plan of intervention for the treatment of the hazardous material in situ. RIASSUNTO. - E noto gia da parecchio tempo che i materiali fibrosi classificati genericamente come *Phone: , fax: , asbesti (appartenenti alia famiglia del serpentino nella varieta crisotilo ed alia famiglia dell'anfibolo varieta riebeckite e grunerite) sono potenziali agenti cancerogeni. Data la presenza a tutt' oggi sui territorio di milioni di m2 di prodotti quali il cementoamianto o I' ami an to fioccato contenenti percentuali variabili da 0.5 a 20% in peso di asbesto, la caratterizzazione di questi materiali per una corretta classificazione e trattamento, e condizione essenziale per qualsiasi tipo di intervento. La diffrazione di raggi X su polveri si e dimostrata, ancora una volta, strumento fondamentale per la caratterizzazione in bulk dei materiali. La tecnica che ven a descritta si avvale della combinazione del metodo Rietveld e del metodo RIR (Reference Intensity Ratio) per arrivare alia determinazione quantitativa di asbesto in materiali massivi contenenti fibre di Iana di vetro (materiale amorfo). Nel presente lavoro viene descritta in particolare I' applicazione per la risoluzione di un problema reale legato alia bonifica in situ di amianto fioccato presente all'universita di Jussieu (Parigi, Francia). KEY WoR DS: Asbestos, chrysotile, grunerite, c01nbined Rietveld-RIR method, loose asbestos containing materials, epoxy resin.
2 2 A.F. GUALTIERI INTRODUCTION Asbestos minerals are classified in amphibole species (anthophyllite, grunerite or mnosite, riebeckite or crocidolite and tremolite) and serpentine species: lizardite (Rucklidge and Zussman, 1965), antigorite (Kunze, 1961 ), chrysotile (Whittaker, 1956), and carlosturanite (Mellini et al., 1985). Asbestos fibers have been utilised since antiquity: anthophyllite for example was used in pottery in Finland in 2500 B.C., clothes made of asbestos were described by Carlemagne in 800 A.D. and Marco Polo in 1250 A.D. (Liddell, 1991). Major industrial use of asbestos began in 1878 with mining of chrysotile in Quebec (Canada) followed by crocidolite mining in 1910 and amosite mining in 1916 in South Africa. After more than 30 years, toxicity of asbestos was recognised: Doll in 1995 in fact observed increased mortality from lung cancer in British asbestos workers (Bhandari and Dhariyal, 1990). In 1972, in USA it was established a Permissible Exposure Limit (PEL) for asbestos of 2.0 fibres/ml (f/ml) as an 8-hour-time-weighted average (TW A) and in 1986 PEL was reduced to 0.2 flml. Currently there is ongoing concern about the health risks associated with exposure to asbestos since exposure to asbestos fibres is associated with diseases like asbestosis, mesothelioma, lung cancer. Concerning the hazardous effects, it is well known that surface features and physical shape of the asbestos particles play a key role in the interaction with the organism cell interface (Hochella, 1993; Langer et al., 1972; Johan et al., 1976; Thomassin et al., 1976; Jurand et al., 1983). According to Hume and Rimstidt (1992) the dissolution reaction of chrysotile in the ph range of lung fluids is: Mg 3 Si205(0H)4 + 6H+ 3Mg H4Si04 + H20. From this, they predicted that a 1 11m diameter chrysotile fibre would completely dissolve in the human lung in 9.0(4.5) months. Therefore, because the onset of disease is generally long (20 years), at least the first step in disease generation should be relatively quickly (Hoc ell a, 1993; Pott, 1987). From epidemiological and in vivo studies, it is clear that crocidolite fibres have a remarkably longer lifetime in the lung tissue than chrysotile (Jones et al., 1989) and thus more pathogenic than chrysotile since they seem relatively chemically stable in lung-like environments (Harington, 1962; Kane, 1993; Stanton et al., 1981). In addition, amphibole asbestos is more hazardous than chrysotile because it contains iron. In fact, hydroxyls and super-oxide free radicals as generated by catalysis on fibre surfaces and the toxic hydroxyl radicals are generated in the presence of free oxygen. The mechanism involves the reduction of oxygen via the oxidation of iron on the mineral surface and the basic equation is (Fenton, 1984): H202 + Fe2 + OH + OH - + Fe 3 + Regarding the physical shape, the activity among the different fiber types increases with decreasing diameter and increasing fibre length (Ross et al., 1993). Stanton et al. (1981) postulated that the optimum morphology for the induction of intrapleural cancer is a diameter of m and a length >8 flm. Concerning the cytoxicity, a number of in vitro and in vivo studies were carried out in the past but still a general picture is not clearly drawn. Because macrophages are avidly phagocytic, mineral particles are rapidly internalised, and macrophages release a diverse array of products (inflammatory activity) into their extracellular environment and stimulate oxidant production (Nathan, 1987). Alternatively, macrophages and neutrophils produce a number of enzymes, oxidants, chemo-attractants and cytokines (particularly TNF-a) which may: a) deactivate minerals; b) activate cell defense mechanisms; c) cause cell injury and abnormal cell function of epithelial cells, fibroblasts, and mesothelial cells, that is, they can initiate or take part to the disease process (Fenton, 1984; Weitzmann and Graceffa, 1984). The need of a characterisation and accurate
3 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 3 quantitative analysis of asbestos containing materials is of key importance for a number of reasons: (a) classification of the material typology and definition of the hazardousness degree for the application of new restrictive laws imposed by the environmental agencies (Veblen and Wylie, 1993); (b) classification of the material typology for a proper plan of intervention and disposal; (c) understanding of the interaction asbestos-organism in biological studies. The application of the Rietveld method to poorly crystalline mixtures containing disordered phases such as chrysotile is not possible. The Rietveld method is successful for the extraction of quantitative data when the structure of the crystalline phases in the mixture is ordered or has a limited extent of disorder. The structure of chrysotile is described as a cylindrical lattice, and has a large density of structure disorder. This causes reflections along well defined crystallographic directions to be broadened. In such conditions, the integrated intensity of the modulated bands as simulated in the Rietveld-type refinements are underestimated with respect to the observed profiles, and therefore the value of the phase fraction obtained from the Rietveld refinement leads to an incorrect amount of chrysotile. Gualtieri and Artioli (1995) developed a reliable structure model for the disorder in chrysotile. Without such a model, the application of the Rietveld method (Rietveld, 1969; Bish and Post, 1993; Young, 1993) is not possible. However, the developed model cannot fully account for the broadening of the diffraction peaks and therefore an internal normalisation by RIR (Reference Intensity Ratio) (Davis et al., 1990) is required. The combined Rietveld-RIR method offers a number of advantages: (a) it is based on a rigorous model for the structure of chrysotile; (b) the profile-fitting technique allows control and evaluation of all microstructural, instrumental, and textural parameters of the sample, so that the proposed structure model can be adopted to chrysotiles with different degree of disorder; (c) the phase fractions extracted by the Rietveld refinements are rescaled on the basis of the absolute weight of corundum originally added to the mixture as an internal standard (internal renormalization); (d) the technique is of straightforward application and advantageous in terms of sample preparation and time requirements. Since 1994, large areas of the University of Jussieu in Paris have been evacuated because it was unambiguously discovered that the framework of the building is composed of an asbestos rich material. This paper reports the description of the characterisation of the asbestos rich material collected at the building of the University of Jussieu in Paris (France) and a possible plan of intervention for the treatment of the hazardous material in situ. METHODS Theoretical background and previous studies. Chrysotile is described in terms of a cylindrical lattice (Wicks and O'Hanley, 1988; Titulaer et al., 1993). The description of the structure symmetry in the various chrysotile types is rather complex due both to the curvature of the lattice and to the statistical stacking of the layers. Since there is no univocal model for the chrysotile structure and its polytypes, Gualtieri and Artioli ( 1995) developed a structure model capable to satisfactorily describe the diffraction effects in the powder spectrum. The model was developed using the powder diffraction spectrum of the well characterised chrysotile from Jeffrey Mine, Quebec Canada. The structure was refined in space group C2/m, and the effect of layer curvature was modelled by a broadening parameter on the crystallographic direction b. Fig. 1 (after Gualtieri and Artioli, 1995) shows the calibration curves of the expected versus observed chrysotile content using the results of the Rietveld refinement alone (a), and using the RIR corrected values (b). In both cases the samples having different matrix composition lie on the same curve, indicating that the matrix effects have been perfectly accounted for.
4 4 A.F. GUALTIERI expected chrysotile (wt0/o) Fig. 1 - The calibration curves of expected vs observed chrysotile content (wt%) for the reference mixtures: (a) using the weights from the Rietveld refinements. The empty triangles are the ternary mixtures CH 1-CH8; (b) using the weights from the Rietveld refinements and RIR-renormalization. The empty squares are the ternary mixtures CH1-CH8, the empty circles are the CH9 and CHlO multicomponent mixtures (After Gualtieri and Artioli, 1995). Materials and experiments. Two samples from the building of the University of Jussieu in Paris (France) were analysed. The specimen la be led PARIS 1 was sampled from a ceiling of the building; the sample labeled P ARIS2 was sampled from a wall of the building. The samples were considered representative of the construction material of the building. A qualitative investigation by X-ray powder diffraction revealed that the sample PARIS 1 is composed mainly of amorphous material (rock or slag wool) with minor amounts of serpentine asbestos (chrysotile), calcite and brucite. The sample P ARIS2 is as well composed mainly of amorphous material (rock or slag wool) with minor amounts of grunerite, calcite and quartz. For the quantitative analysis, the powders were added 1 O%wt NIST standard corundum to carry out the Rietveld-RIR. Data were collected using a Philips Bragg-Brentano diffractometer with a curved pirolitic graphite monochromator on the diffracted beam, in the range 5-l with steps of , 10 s/step, 0.5 divergence slit, 0.1 mm receiving slit, and 0.5 antiscatter slit. Data sets were refined by the Rietveld method using GSAS (Larson and von Dreele, 1999). In GSAS, the structure factors were calculated by using the formal atomic scattering factors. The background was successfully fitted with a Chebyshev function with 16 coefficients. The peak profiles were
5 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 5 t<) w 0 o X Ca Co + cts L[) theta X10E 2 sample class B Gr Co Q ea theta X10E 2 Fig. 2- The observed and calculated patterns, and difference curve of the refinement of samples PARIS I (a) and PARIS2 (b).
6 6 A.F. GUALTIERI modelled using a pseudo-voight function with one gaussian and one lorenzian coefficient. The lattice constants, the phase fraction, and coefficients corresponding to sample displacement and asymmetry were also refined. The total number of parameters refined at the same time in the last stages of the refinements for each pattern was 40. The SEM (Scanning Electron Microscopy) analysis of the sample was performed on specimens of ea. 0.7x0.7x0.7 cm mounted on an AI holder and fixed with an Ag paste. Dehydration was performed under an IR lamp for 15 min and coating was performed using Au. A Philips XL 40/604 automated instrument was utilised with a vacuum of ea. I0-7 torr. In order to give a statistical significance to the observations, 20 frames were collected for each specimen. Frames were collected using a beam size of 5 mm and an intensity of 25 k V. RESULTS AND DISCUSSION Fig. 2a and 2b show the observed (crosses), calculated (continuous line) and difference curve (bottom line) of the refined patterns. A good agreement between the calculated and observed patterns is evident at low angle as well as at high angle. The agreement factors for the Rietveld refinements are: Rwp=9% and x 2 =2.1 for PARIS! and Rwp= ll% and x 2 =3.1 for PARIS2, respectively. The results of the quantitative analysis of the two samples are reported in Table 1. Fig. 3 shows the raw samples from the wall (a) and ceiling (b) of the University. PARIS I is composed of an intergrowth of free glass fibers (slag wool) and asbestos fibers plus some grains of crystalline material (mainly calcite). PARIS2 is composed of amphibole asbestos fibres interdispersed in a matrix of glass fibres. Qualitatively fibres looking rigid and brittle are glassy wool, fibres which are rolled with an hair-like shape are asbestos fibres. As it was expected the content of asbestos phases is larger than the maximum amount allowed by law. Thus, the whole building was reasonably evacuated in 1994 and a drastic plan of intervention is demanded. Among the various solutions, the neutralisation of the asbestos containing material can be performed in situ by spraying an epoxy resin on walls and ceiling which is capable to penetrate and cement the fibres, preventing its dispersion in air. Such intervention was described in detail in Gualtieri (1998) and Gualtieri (1999). TABLE 1 Results of the quantitative analysis of the samples PARISJ and PARIS2. phase Parisl Paris 2 Chrysotile 6.3(6) Grunerite 9.5(9) Brucite 0.6(2) Calcite 6.7(5) 5.0(6) Quartz 0.5(2) Glass 86(1) 85(1)
7 The aid ofx-ray pmvder diffi action to the characterisation and treatment of asbestos containing materials = 5 I-'ll a b = 21-'m Fig. 3 - SEM image of the untreated specimen sampled at the University of Jussieu Paris. Sample (a) is PARIS l, sample (b) is PARIS2.
8 8 A.F. GUALTIERI a = 5 f..!m b = 1 f..! m Fig. 4 - SEM magnified images of PARIS 1 after the interaction with the epoxy resin at a different magnification showing a clear change in the microstructure of the material.
9 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 9 As discussed by Harington (1962), hemolitic activity of chrysotile asbestos is blocked by chelators, particularly those with affinity for Mg. There are a number of groups that may modify the surface chemistry of chrysotile fibers to reduce they cytoxicity. Although the monoionic polymer polyvinyl-2-pyridine N oxide (PVPNO) does not passivate chrysotile, some ecidic, water soluble polymers, such as carboxymethylcellulose (CMC) are effective (Schnitzer, 1974). Brown et al. (1990) published a report in which they describe the modification of the surfaces of amosite fibers (mostly cummingtonite-grunerite) with octyldimethyl-chlorosilane (C8) or octadecylmethylchlorosilane (C18) through in vivo studies showing that fibers coated with C 18 chains were dramatically less active at producing tumors. Besides, Pott et al. ( 1989) reports that actinolite with 2-polyvinylpyridine N-oxide hydrogen bonded to its surface produced fewer mesotheliomas with a longer latency period than actinolite without polymer. For these reasons the utilisation of an epoxy resins should also benefit for the neutralisation of the surface activity of asbestos. The investigated specimen were treated by epoxy resin (see description in Gualtieri 1999) and observed by SEM after the treatment in order to put into evidence the differences in the morphology and microstructure of the materials before and after the interaction with the epoxy resin. Fig. 4a,b are magnified image of PARISl after the treatment with the epoxy resin. It is evident a change in the micro-structure of the material which is now a diphasic material where the fibres and the crystals are now cemented by the resin. Fibres are thus captured in a solid matrix which inhibits the dispersion in air medium. The same applies for sample PARIS2 (fig. 5) = 2 jlm Fig. 5 - SEM magnified images of PARIS2 after the interaction with the epoxy resin.
10 10 A.F. GUALTIERI It is possible to say that a proper in situ intervention using an epoxy resin modifies the nature of the asbestos containing materials which do not release free fibres in air and thus restore a safe environment to the scientific community of the University. A plan of intervention on an industrial scale has been proposed by AXSON Technologies, a France enterprise which produces the epoxy resin for the treatment. The purpose is still under discussion by the France Government. CONCLUSIONS In the present work we successfully applied the combined Rietveld-RIR for the quantification of chrysotile asbestos in bulk materials from the main building of the University of Jussieu (Paris, France). The addition of an internal standard (RIR) is necessary to overcome the matrix (glassy, clay, heterogeneous) effects and better account for the structural disorder of chrysotile. The importance of the study is paramount for either intervention plans and biological studies. It was demonstrated that a proper intervention in situ with an epoxy resin modifies the nature of the asbestos materials which do not release free fibres in air and thus restoring a safe environment. In the specific case, quantitative characterisation of the material is necessary for the development of the proper composition of the epoxy resin since composition is terms of viscosity and solvent addition is strictly dependent upon the mineralogical composition. ACKNOWLEDGEMENTS AXSON Technologies and ST AC Roofing srl are acknowledged for permission of making experimental data on the PARIS project available. Grants were obtained from Italian C.N.R. and M.U.R.S.T. REFERENCES BHANDARI, R.K. and DHARIYAL, K.D. (1990) Asbestos and associated health hazards, Central Building Res. Inst. Roorkee, Oxford and IBH Pub. Co. PVT. LTD New Delhi, 54 pp. BISH, L.B. and PosT, J.E. (1993) - Quantitative mineralogical analysis using the Rietveld fullpattern fitting method. Am. Min., 78, BROWN, R.C., CATHEW, P., HOSKINS, J.A., SARA, E., and SIMPSON, C.F. (1990) - Swface modification can affect the carcinogenicity of asbestos. Carcinogenesis, 11, DAVIS, B.L., KATH, R., and SPILDE, M. (1990) The reference Intensity ratio: Its measurenlent and significance. Powder Diff., 5, FENTON, H.J.H. (1984) - Oxidation of tartaric acid in presence of iron. J. Chem. Soc., 65, GUALTIERI A.F. and ARTIOLI G. (1995) - Quantitative determination of chrysotile asbestos in bulk materials by combined Rietveld and RIR methods, Powder Diffraction, 10(4), GUALTIERI A.F. (1998) - A solution to the asbestos problem: the in situ impregnation by an epoxy resin. Reunion «Le traitment de l'amiante in situ» Press Club de France, Paris, 29 giugno GUALTIERI A.F. (1999) -A solution for the full impregnation of asbestos: the use of an epoxy polymer resin, J. App. Polymer Science, submitted. HARINGTON, J.S. (1962) -Natural occurrence of oils containing 3,4-benzpyrene and related substances in asbestos. Nature, 193, HOCHELLA, M.F. (1993) - Surface chemistry, structure, and reactivity of hazardous mineral dusts. in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, HUME, L.A., and RIMSTIDT, J.D. (1992) - The biodurability of chrysotile asbestos. Am. Min., 77, JOHAN, Z.A., GONI, J., SARCIA, C., BONNAUD, G., and BIGNON, J. (1976) - Influences de certains acides organiques sur la stabilite du reseau du chrysotile. 6th Cong. Int. Geoch. Organique Technip. Ed. Paris, JoNES, A.D., VINCENT, J.H., MciNTOSH, C., MACMILLAN, C.H., and ADDISON, J. (1989) - The effect of fiber durability on the hazard potential of inhaled chrysotile asbestos fibers. Exper. Path., 37, JURAND, M.C., BIGNON, J., SEBASTIEN, P., and GONI, J. (1983) - Leaching of chrysotile asbestos in human lungs. J. Colloid. Interf. Sci.», 95, 1-9. KANE, A.B. (1993) - Epidemiology and pathology of asbestos-related diseases, in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, KUNZE, G. (1961) - Antigorit. Strukturtheoretische Grundlangen aun ihre praktische bedetung fiir die
11 The aid of X-Ray powder d(ffraction to the characterisation and treatment of asbestos containing materials 11 weiters serpentin-forschung, Fortschr. Min. 39, LANGER, A.M., RUBIN, l. B., SELIKOFF, I.J., and POOLEY, F.D. (1972)- Chemical characterization of asbestos baby cores by electron microprobe analysis. J. Hystochem. Cytochem., 20, LARSON A.C. and VON DREELE R.B. (1999) GSAS: General structure analysis system. Report LAUR Loa Alamos National Laboratory, NM 130 pp. LIDDELL, D. (1991) - Exposure to mineral fibers and human health: historical backgroud. In Mineral fibers and health, D. Liddell and K. Miller Eds. Boca Ratan CRC Press Florida Cap 1. MELLINI, M., FERRARIS, G. and COMPAGNONI, R. (1985) - Carlosturanite: HRTEM evidence of a polysomatic series including serpentine. Am. Min., 70, NATHAN, C.F. (1987) -Secretory products of macrophages. J. Clin. Invest., 79, POTT, F. (1987) - Problems in defining carcinogenic fibres. Ann. Occup. Hygiene», 31, PoTT, F., RoLLER, M., ZIEM, U., REIFFER, F.J., BELLMANN, B., ROSENBRUCH, M., and HUTH, F. (1989) - Carcinogenicity studies of natural and man-made fibers with the intraperitoneal test in rats. in Non occupational exposure to mineral fibers. Bignon, J. Ed. IARC Sci. Publ. No 90, Lyon France, RIETVELD, H.M. (1969) -A profile refinement for nuclear and magnetic structures. J. App. Cryst., 2, Ross, M., NOLAN R.P., LANGER, A.M., COOPER, W.C. (1993) -Health effects of mineral dusts other than asbestos. in «Health effects of mineral dusts». G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am., 28, pp RUCKLIDGE, J.C. and ZUSSMAN, J. (1965) -The crystal structure of the serpentine mineral lizardite Mg3Si205(0H)4, Acta Cryst., 19, SCHNITZER, R.J. (1974) -Modification of biological swface activity of particles. Environ. Health Oers., 9, STANTON, M.F., LAYARD, M., TEGERIS, A., MILLER, E., MAY, M., MORGAN, E., SMITH, A. (1981) - Relation of particle dimension to carcinogenicity of amphibole asbestos and other fibrous minerals. J. Nat'l Cancer Inst., 67, THOMASSIN, H., GONI, J., BAILLIF, P., TOURAY, J.C. (1976) -Etude par spectrometrie ESCA des premiers stades de la lixiviation du chrysotile en milieu acide organique. C. R. Acad. Sci. Paris, 283, TITULAER, M.K., VAN MILTEBURG, J.C., JANSEN, J.B., and GEus, J.W. (1993) - Characterization of tubular chrysotile by thermoporometry, nitrogen sorption, drifts and TEM. Clays and Clay Min., 4, VEBLEN, D.R. and WYLIE, A.G. (1993) - Mineralogy of amphiboles and 1:1 layer silicates. in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, WEITZMAN, S.A., and GRACEFFA, P. (1984) Asbestos catalyzes hydroxyls and superoxide radicals generation from hydrogen peroxide. Arch. Biochem. Biophys., 228, WHITTAKER, E.J.W. (1956) -The structure of chrysotile. I!. Clinochrysotile. Acta Cryst., 9, WICKS, F.J., and O'HANLEY, D.S. (1988) - Serpentine minerals: structures and petrology. in Hydrous Phyllosilicates S.W. Bailey ed. Min. Soc. of Am. 19, YouNG, R.A. (1993). The Rietveld method. Oxford University Press, 235 pp.
DOI: 10.2451/2013PM0018 PERIODICO di MINERALOGIA established in 1930 An International Journal of MINERALOGY, CRYSTALLOGRAPHY, GEOCHEMISTRY, ORE DEPOSITS, PETROLOGY, VOLCANOLOGY and applied topics on Environment,
Boulanger et al. Environmental Health 2014, 13:59 REVIEW Open Access Quantification of short and long asbestos fibers to assess asbestos exposure: a review of fiber size toxicity Guillaume Boulanger 1,
1 Asbestos as a metaphor for teaching risk perception (modified slightly from Gunter, M.E. (1994) Journal of Geological Education, 42, 17-24) ABSTRACT Asbestos -- the word means different things to different
An Evaluation of the Risks of Lung Cancer and Mesothelioma from Exposure to Amphibole Cleavage Fragments John F. Gamble, Ph. D. International Environmental Research Foundation Post Office Box 3459 Grand
Asbestos exposure and disease: notes for medical practitioners This pamphlet has been developed from the Asbestos Advisory Committee's report to the Minister of Labour on medical and industrial issues.
Asbestos Risks of environmental and occupational exposure G e z o n d h e i d s r a a d H e a l t h C o u n c i l o f t h e N e t h e r l a n d s To the Minister of Housing, Spatial Planning and the Environment
AMERICAN JOURNAL OF INDUSTRIAL MEDICINE (2009) Historical Perspective Developments in Asbestos Cancer Risk Assessment Michael A. Silverstein, MD, MPH, 1 Laura S. Welch, MD, 2 and Richard Lemen, PhD, MSPH
THE ASBESTOS DILEMMA: 1. ASSESSMENT OF RISK Fedor VALIC Andrija Stampar School of Public Health, Medical Faculty University of Zagreb, Zagreb, Croatia Received March 2002 Arh Hig Rada Toksikol 2002; 53:
Critical Reviews in Toxicology, 38(S1):49 73, 2008 Copyright c 2008 Informa UK Ltd. ISSN: 1040-8444 print / 1547-6898 online DOI: 10.1080/10408440802273156 A Meta-Analysis of Asbestos-Related Cancer Risk
The risk of mesothelioma from exposure to chrysotile asbestos Charles M. Yarborough Purpose of review This review assesses the risk of developing diffuse malignant mesothelioma of the pleura from exposures
EUROPEAN COMMISSION DIRECTORATE-GENERAL HEALTH AND CONSUMER PROTECTION Directorate C - Scientific Opinions Unit C2 Management of Scientific Committees; scientific co-operation and networks Scientific Committee
Asbestos exposure in New Zealand: Review of the scientific evidence of non-occupational risks A report on behalf of the Royal Society of New Zealand and the Office of the Prime Minister s Chief Science
American Thoracic Society Documents Diagnosis and Initial Management of Nonmalignant Diseases Related to Asbestos This official statement of the American Thoracic Society was adopted by the ATS Board of
MINISTRY OF CHEMICALS AND FERTILISERS, GOVT. OF INDIA SPONSORED PROJECT Study of Health hazards / Environmental hazards resulting from use of Chrysotile variety of Asbestos in the country NATIONAL INSTITUTE
Home Search Collections Journals About Contact us My IOPscience Heterogeneity of exposure and attribution of mesothelioma: Trends and strategies in two American counties This content has been downloaded
PROGRAMME OBJECTIVE SERIES: PROBES/123/2008 2009 HUMAN HEALTH RISK ASSESSMENT STUDIES IN ASBESTOS BASED INDUSTRIES IN INDIA CENTRAL POLLUTION CONTROL BOARD (MINISTRY OF ENVIRONMENT AND FORESTS) Website
Asbestos on ships How to manage it safely Lloyd s Register Group Limited, its affiliates and subsidiaries and their respective officers, employees or agents are, individually and collectively, referred
J Mater Sci (2007) 42:2917 2933 DOI 10.1007/s10853-006-0637-z ADVANCES IN GEOPOLYMER SCIENCE & TECHNOLOGY Geopolymer technology: the current state of the art P. Duxson Æ A. Fernández-Jiménez Æ J. L. Provis
Asbestos Exposure Risk Assessment Endeavour Energy Residential Houses Electrical Boxes around Western Sydney NSW November 2012 Our Ref: C107533: J115323 Noel Arnold & Associates Pty Ltd Office 2, 120 Smith
InformatlDn Act: Document dlvulgue en vertu de la LOIsur iacces a i Information. 1+1 Health Sante Canada Canada Chrysotile Asbestos Consensus Statement and Summary Chrysotile Asbestos Expert Panel Montreal,
CODE OF PRACTICE FOR THE MANAGEMENT AND CONTROL OF ASBESTOS IN WORKPLACES [NOHSC: 2018 (2005)] CANBERRA APRIL 2005 NATIONAL OCCUPATIONAL HEALTH AND SAFETY COMMISSION CODE OF PRACTICE FOR THE MANAGEMENT
Technical Guidance for the Calculation of Asbestos-Related Risk in Soils for the Basic Management Incorporated (BMI) Complex and Common Areas Prepared For: Nevada Division of Environmental Protection Bureau
Asbestos General information Key Points Fire Non flammable and non combustible under normal conditions Chemically inert under normal conditions. Resistant to most solvents, acids and alkalis In the event
The Management of Asbestos in the Non-occupational Environment Revised edition 2013 Guidelines for Public Health Units Citation: Ministry of Health. 2013. The Management of Asbestos in the Non-occupational